Helicity dependent photocurrent in electrically gated (Bi, Sb ...https:// › publication › fulltexthttps:// › publication › fulltextby Y Pan · 2017 · Cited by 45 — Finally, we find that the HDPC varies dramatically with photon energy, reversing sign at a .
arXiv:1706.04296v1 [cond-mat.mtrl-sci] 14 Jun 2017
Richardella1 , Haijun Zhang3 , David D. Awschalom2 , Chao-Xing Liu1 , Nitin Samarth?1
Department of Physics and the Materials Research Institute, The Pennsylvania State University,
University Park, Pennsylvania 16802-6300, USA 2
Institute for Molecular Engineering, University of Chicago, Chicago, IL 60637, USA
National Laboratory of Solid State Microstructures, School of Physics and Collaborative Innova-
tion Center of Advanced Microstructures, Nanjing University, Nanjing 210093, China
Circularly polarized photons are known to generate a directional helicity-dependent photocurrent in three-dimensional topological insulators at room temperature. Surprisingly, the phenomenon is readily observed at photon energies that excite electrons to states far above the spin-momentum locked Dirac cone and the underlying mechanism for the helicitydependent photocurrent is still not understood. We resolve the puzzle through a comprehensive study of the helicity-dependent photocurrent in (Bi1−x Sbx )2 Te3 thin films as a function of the incidence angle of the optical excitation, its wavelength and the gate-tuned chemical potential. Our observations allow us to unambiguously identify the circular photo-galvanic effect as the dominant mechanism for the helicity-dependent photocurrent. Additionally, we use an analytical calculation to relate the directional nature of the photocurrent to asymmetric optical transitions between the topological surface states and bulk bands. The insights we
obtain are important for engineering opto-spintronic devices that rely on optical steering of spin and charge currents.
Narrow band gap semiconductors such as the Bi-chalcogenides have attracted much contemporary interest as three-dimensional (3D) "topological insulators" (TIs) that host gapless spintextured surface states which reside within the bulk band gap.1–7 The spin-momentum locking in these helical Dirac states provides a unique opportunity for “topological spintronics" devices that function at technologically relevant temperatures (300 K and above).8–10 Optical methods have also been adopted to control electron spin and charge currents in 3D TIs.11–14 In particular, experiments have shown that circularly polarized light induces a directional helicity-dependent photocurrent (HDPC) in 3D TIs: in other words, light of opposite circular polarization yields a photocurrent propagating in opposite directions.15 The ready observation of this phenomenon at 300 K promises interesting opportunities for developing opto-spintronic devices wherein electron currents might be steered optically. Progress toward such technological applications is however impeded by a lack of understanding about the physics underlying this phenomenon.
The natural impulse is to immediately attribute the HDPC in 3D TIs to the helical spin texture of the Dirac surface states:15 circularly polarized photons couple to the spin-momentum locked topological surface states, yielding a circular photo-galvanic effect (CPGE), a phenomenon well-established in semiconductor quantum wells, where the inversion symmetry breaking is the cause.16, 17 Time-resolved measurements of the HDPC in 3D TIs seem to confirm the surfacerelated origin for the HDPC by showing that the group velocity of the induced photocurrent
matches that expected for Dirac surface electrons.18 However, this interpretation is difficult to reconcile with the fact that the photon energy used in the experiments is about 5 times larger than the bulk energy gap. This means that the optical transitions involved in creating photo-electrons cannot involve the Dirac surface states alone.
In principle, HDPC can also be generated by the photon drag effect which involves the transfer of both spin angular momentum and translational momentum from circularly polarized photons to electrons.19–21 It is thus relevant to develop an experimental test that distinguishes between CPGE and photon drag as the origin of the HDPC. Another relevant question is the underlying microscopic mechanism for the HDPC. While both the CPGE and the photon drag effect can be related to optical transitions involving the lowest energy surface states alone, there are several other possibilities. These include the asymmetric scattering of electrons,22 a “surface shift current,"23 a photocurrent arising from Rashba states,24–26 and a photocurrent arising from excitation into the second excited band of surface states.18, 27 So far, there have been very few attempts to clearly rule out any of these alternative interpretations.
Here, we describe a comprehensive experimental study of the HDPC in thin films of an electrically gated 3D TI ( (Bi1−x Sbx )2 Te3 ). By revealing three prominent features in the behavior of the HDPC, we unambiguously identify its physical and microscopic origin:
1. We find that the HDPC varies as sin θ, where θ is the angle of incidence of the excitation. 2. By tuning the carrier density with a top gate, we find that the HDPC is a non-monotonic
function of the chemical potenti